- Email: [email protected]

Contents lists available at ScienceDirect

Journal of Natural Gas Science and Engineering journal homepage: www.elsevier.com/locate/jngse

Modeling of nitrogen separation from natural gas through nanoporous carbon membranes Abdulrahman A. Al-Rabiah a, *, Abdelhamid M. Ajbar a, Moustafa A. Soliman a, b, Fahad A. Almalki c, Omar Y. Abdelaziz d a

Chemical Engineering Department, King Saud University, Riyadh 11421, Saudi Arabia Department of Chemical Engineering, The British University in Egypt, El-Shorouk City, Cairo 11837, Egypt King Abdulaziz City for Science and Technology, Riyadh 11442, Saudi Arabia d Department of Chemical Engineering, Cairo University, Giza 12613, Egypt b c

a r t i c l e i n f o

a b s t r a c t

Article history: Received 2 July 2015 Received in revised form 20 August 2015 Accepted 20 August 2015 Available online 25 August 2015

This work presents a theoretical investigation of the use of nanoporous carbon membranes for the separation of nitrogen from natural gas. A mathematical model to predict the performance of the membrane is developed. The model is a combination of the well known dusty gas model, which describes the transfer of multi-components mixture in porous media, together with a surface diffusion model. The model is ﬁrst validated using the literature results for the separation of hydrogen from hydrocarbons mixture. The model is then applied to the nitrogen-hydrocarbons system. The membrane performance is evaluated in terms of nitrogen recovery, methane loss, nitrogen purity, as well as hydrocarbons compositions in both permeate and retentate sides. The model calculation methods are applied for both co-current and counter-current ﬂow conﬁgurations. A parametric study is also carried out to investigate the effects of membrane parameters such as feed and permeate pressures and porosity on the membrane performance. The developed model is general and can be applied to various nanoporous membrane ﬂow patterns. © 2015 Elsevier B.V. All rights reserved.

Keywords: Nanoporous carbon membrane Dusty gas model Mathematical modeling Nitrogen removal Natural gas Selective surface ﬂow

1. Introduction Natural gas is of great importance as a primary source of energy, synthesis gas and as a raw material for petrochemical industries. Ammonia and methanol are examples of industries that beneﬁt from the natural gas as a raw material. Most industrial speciﬁcations require no more than 4% nitrogen or total inerts in the pipelines (Baker, 2002). Large proven reserves in the world cannot be produced due to presence of high percentage levels of nitrogen gas. The Kingdom of Saudi Arabia, for instance, has one of the world's highest proven reserves of natural gas. As reported by Saudi Aramco, it is estimated at 241 trillion cubic feet, ranking fourth in the world after Russia, Iran, and Qatar (Aleklett et al., 2010). About 60% of these reserves are “associated gas” from oil ﬁelds. Most of Saudi Arabia's non-associated gas reserves contain mainly methane and a high nitrogen content that normally exceeds 14 mol %. Technology is therefore needed to economically bring the gas to pipeline

* Corresponding author. E-mail address: [email protected] (A.A. Al-Rabiah). http://dx.doi.org/10.1016/j.jngse.2015.08.040 1875-5100/© 2015 Elsevier B.V. All rights reserved.

quality levels. Currently, there are essentially four possible methods available for removal of nitrogen from natural gas: cryogenic distillation, pressure swing adsorption (PSA) process, lean oil absorption processes, and membrane processes. The cryogenic process is the only process that is used nowadays on any industrial scale. PSA process is of limited commercial application, while the remaining processes are in the research stage. Cryogenic processes are typically used with large capacity applications. The process is characterized by a high methane recovery rate. However, high capital and compression costs besides the need for extensive pretreatment are major drawbacks within the process. The pretreatment consists generally of amine scrubbing in order to remove the carbon dioxide present. Next, glycol dehydration is performed to eliminate most of the water vapor. Molecular sieves afterward get rid of any carbon dioxide and water vapor left, after which the gas is chilled in a ﬁnal polishing stage to eliminate heavy hydrocarbons and aromatics. The complexity of the pretreatment makes the operational reliability a concern. On another hand, methane and other hydrocarbons are commonly adsorbed onto molecular sieves in the PSA

A.A. Al-Rabiah et al. / Journal of Natural Gas Science and Engineering 26 (2015) 1278e1284

process, resulting in a nitrogen-rich gas stream (Tagliabue et al., 2009). Typically, multiple beds are employed, with complex switching controls across the beds. However, the capital and operating costs of these systems are rather high. Meanwhile, lean oil absorption processes have been under establishment for about 20 years (Yildirim et al., 2012). Such processes mostly exploit chilled oil to absorb methane and other hydrocarbons. A good recovery for hydrocarbons is attained, but the process is often considered capital intensive. Also, the requirement to absorb methane bulk further increases equipment size and compression duties. It is expected in the upcoming decades that, more efﬁcient nitrogen removal technologies will emerge to improve the materials stability and the separation power (Rufford et al., 2012). Membrane technology has been considered recently for gas separation (Ahmad et al., 2015; Bara et al., 2009; Cai et al., 2012; Rezakazemi et al., 2011; Saidi et al., 2014) and nitrogen removal from natural gas (Baker et al., 2003; Lokhandwala et al., 2010; Wu et al., 2015). The use of membranes offers in general a number of advantages including low capital cost, low energy use, cost effectiveness even at low gas volume, and considerable weight and space efﬁciency (Scholes et al., 2012). For the nitrogen removal from natural gas, either glassy polymers that are ordinarily nitrogen-permeable, or rubbery polymers that are normally methane-permeable, can be used. Ever since, these traditional polymeric membranes (glassy and rubbery) have low selectivities for nitrogen over methane and vice versa (Baker et al., 2003). On the other hand, inorganic membranes, including nanoporous membranes, have the desirability of higher permeability values comparing to polymeric membranes, and their selectivities are however high (Baker, 2002). Table 1 shows a comparison between different membrane materials that can be adopted for nitrogen removal from natural gas. Carbon porous membranes appeared to provide added features comprising higher rates of transport, thermal stability, and high selectivity. Two types of carbon membranes have acquired much attention for gas separation: namely, molecular sieving membranes and nanoporous membranes (Seo et al., 2002). In molecular sieving membrane, the separation is based on molecular size differences (Koresh and Sofer, 1983). This kind of membranes allows passage of smaller molecules through the pores of the membrane while blocking larger molecules. The molecular sieving membranes can have high permeability and selectivity for the smaller components. Despite of that, they need delicate control of the pore sizes close to the size of the gas molecules to be separated (Seo et al., 2002). In nanoporous membranes, the pores are larger than the dimension of the molecules and the separation selectivity is determined by surface diffusion and preferential adsorption of the more strongly adsorbed species (Vieira-Linhares and Seaton, 2003). Thus, both the pore size and the nature of the surface play key roles in the membrane performance. In their pioneering work, Rao and Sircar (Rao and Sircar, 1993a) developed a nanoporous carbon membrane, which they called selective surface ﬂow (SSF) membrane. This membrane has pore sizes typically in the range of 5e6 Å, and achieved separation on the selective adsorption basis followed by

1279

surface diffusion. Additionally, the authors went further to study the SSF membrane performance for the separation of hydrogenhydrocarbon gas mixtures (Rao and Sircar, 1996). Mathematical modeling of nanoporous membranes has also grabbed an increasing attention in literature (Bowen and Welfoot, 2002; Habib and Habib, 2004; Seo et al., 2002; Vieira-Linhares and Seaton, 2003; Xu et al., 2000). Such tailor-designed membranes are considered to play an important role in improving membrane systems and environment (Dionysiou, 2004). Because of the nanoscale nature of the membrane, molecular dynamics (MD) modeling and Monte Carlo (MC) simulation, have been commonly used in studying the molecular diffusion in porous medium (Seo et al., 2002; Vieira-Linhares and Seaton, 2003; Xu et al., 2000). A number of these modeling studies addressed the permeability and selectivity prediction of nanoporous carbon membranes, but there has been no report on the detailed performance study of nanoporous carbon membranes for nitrogen removal from natural gas. The general objective of this research is to contribute to the understanding of the potential beneﬁts of using nonporous membrane for the nitrogen removal from natural gas through the development of a mathematical model of the membrane and the determination of its performance. The model and calculation methods are presented for both co-current and counter-current ﬂow conﬁgurations. The organization of this paper includes the presentation of the model and the solution strategy for both ﬂow conﬁgurations, proceeding ahead to the validation of the model using the results of the pioneering work of Rao and Sircar (Rao and Sircar, 1996) for hydrogen-hydrocarbons system. This is followed by the presentation of simulation results for nitrogen-hydrocarbons system.

2. Modeling the nanoporous membrane The model developed in this work is used to predict the transport of different species of multi-component gas mixture through the nanoporous membrane. The model includes the following transport modes that exist in porous media: (1) Free-molecule or Knudsen ﬂow, where the gas density is low to the point that collisions between gas molecules can be neglected, contrasted with gas molecules collisions with the walls of porous medium. (2) Viscous or convective or bulk ﬂow, where the gas performs as a continuum ﬂuid forced by a pressure gradient, and gasegas collisions control over gasewall collisions. (3) Ordinary or continuum diffusion, to which the mixtures unlike species move relative to one another affected by concentration gradients. (4) Surface ﬂow or adsorption, in which molecules move along a solid surface in an adsorbed layer (Fuertes, 2000; Rao and Sircar, 1993b). For the development of the model, we consider a similar schematic diagram for the membrane with counter-current ﬂow used by Shindo et al. (Shindo et al., 1985), as shown in Fig. 1. The following are the main assumptions used to derive the mathematical model:

Table 1 Comparison between different membrane materials including the nanoporous carbon membrane (Scholes et al., 2012). Membrane material

Type

Selectivity PCH4/PN2

Selective surface ﬂow (SSF) Polydimethysiloxane (PDMS) PTMSP Polyimide (6FDA-BAHF) Polyamide-polyether block copolymer (Pebax® 2533) Silicon rubber

Nanoporous inorganic Rubbery polymer Super glassy polymer Glassy polymer Rubbery polymer Rubbery polymer

8.80 3.15 2.44 2.3 at PN2/PCH4 2.8 at T ¼ 22 C 4

1280

A.A. Al-Rabiah et al. / Journal of Natural Gas Science and Engineering 26 (2015) 1278e1284

membrane, DK i the Knudsen diffusivity, Dij the binary gas diffusivity, r the pore radius, andmi is the gas viscosity. PN ðxj Ni xi Nj Þ represents the Stefan Maxwell term The term j¼1 Dij

y1

Permeate G

G, y1p,……,yn Feed

yn

-dF

x1

x1+dx1

xn

xn+dxn

Membrane

Ff, x1f,…,xnf

F+dF

Ni DKi

Retentate

(multi-component molecular diffusion), while

Fo, x1o,…,xno

diffusion (moleculesewall interaction). The term

dz

the

ε r2 P t 8 mi DK i

dP dz

is

intra-molecular

P dxi RTL dz

Fig. 1. Membrane ﬂow diagram with counter-current ﬂow.

is the Knudsen !

xi þ RTL

dP dz

1 ¼ RTL

viscous friction, while the term dPxi represents the concentration gradient. dz

The surface diffusion ﬂux is, on another hand, given by Plug ﬂow conditions are assumed in the feed and permeate sides. Permeability is assumed to be independent of pressure and temperature for every gas component. The membrane thickness is assumed to be constant all over the entire length of the unit. Pressure drop is negligible for the feed stream as well as the permeate gas stream. The feed gas is assumed to consist of nitrogen and essentially the following mixture of hydrocarbons: CH4, C2H6, C3H8 and C4H10. The same notations that were used for the development of simple solution-diffusion model are adopted here. This approach is in good agreement and exists with prior literature results for membrane separation processes (e.g., Mulder, 1996; Rao and Sircar, 1996; Wijmans and Baker, 1995).

2.1. Model for co-current conﬁguration We consider the schematic diagram for a membrane (Fig. 1) but with co-current ﬂow. The balance equations for each component (i) are given by:

dFi ¼ NTi ; dA dGi ¼ NTi ; dA

Fi ð0Þ ¼ Ff yi ð0Þ

Gi ð0Þ ¼ 0

i ¼ 1; 2; n

i ¼ 1; 2; n

N X

xi ¼ 1

The model equations are solved using the orthogonal collocation method (Soliman, 1992). The orthogonal collocation is applied at nc interior collocation points inside the membrane such that:

X dxi;j ncþ1 ¼ Ajþ1;k xi;k1 þ Ajþ1;1 yi dz

(6) There are (n nc)variables: x(i þ (j 1)n) i ¼ 1,2, … ,n and j ¼ 1,2, … ,nc where i represents a component and j represents a collocation point. Aj,k are the elements of ((nc þ 1) (nc þ 1)) matrix of the weights of ﬁrst derivative. Similarly, for the pressures:

X dPj ncþ1 ¼ Ajþ1;k P k1 þAjþ1;1 Pf dz

j ¼ 1; 2; nc

(7)

k¼2

(1)

(2)

mi ¼

ncþ1 X

Xinterp k xi;k1 þ Xinterp 1 yi

i ¼ 1; 2; n 1

(8)

In which that (Xinterp)k is the elements of (nc þ 1) 1 vector of weights of the Lagrange interpolation formula at z ¼ 1. Also, we have:

G mi ¼ Pn i

i¼1

(9)

The pressure Pp at the permeate side is, on the other hand, given

Pp ¼

The dusty gas model equations adopted are given as:

Gi

by:

(3)

x ε r2 P þ i 1þ t 8 mi DKi RTL

j ¼ 1; 2; nc and i ¼ 1; 2; :::; n

k¼2

k¼1

NTi ¼ Ni þ NSDi N X xj Ni xi Nj N P dxi Ki ¼ RTL dz Dij Di j¼1

(5)

i¼1

Where Pf is the pressure at feed side and Pk ¼ x(nnc þ k), k ¼ 1,2,..,nc. The mole fractions (mi) regarding the gas at the permeate side are required to be equal to those obtained from extrapolation of the gas mole fraction at the feed side such that:

Such that Ff is the inlet feed ﬂowrate, Fi the ﬂowrate of component (i) in retentate, NTi the total ﬂux through the membrane of component (i), Gi the ﬂowrate of component (i) in the permeate, yi the gas mole fraction at the permeate side, AT the membrane area, and Gi(AT) the given component (i) inlet permeate side ﬂowrate at the total area AT (i.e. sweep gas). The total ﬂux (NTi ) is the sum of the dusty ﬂux (Ni) and the surface diffusion ﬂux NSDi :

i NSDi ¼ QL i dPx where Qi is the permeability of component (i). To the dz model equations is added the consistency relation:

ncþ1 X

Xinterp k Pk1 þ Xinterp 1 Pf

(10)

k¼2

!

We have (n þ 1)nc þ n variables that represent the gas ﬂux. Hence, the numbers of equations are:

dP i ¼ 1; 2; n dz (4)

Where L is the thickness of the membrane, z the dimensionless distance through the membrane, P the total pressure inside the membrane, T the temperature, xi the mole fraction inside the

n nc equations of the dusty gas equations (Eq. (4)) at the collocation points. nc equations of the summation equation (Eq. (5)) at nc collocation points. One equation for the permeate pressure (Eq. (10)). (n 1) equations of the combination of (Eq. (8)) and (Eq. (9)) by eliminating mi but replacing (Eq. (9)) by:

A.A. Al-Rabiah et al. / Journal of Natural Gas Science and Engineering 26 (2015) 1278e1284

N mi ¼ Pn i

(11)

i¼1 Ni

Consequently, this gives a total of (n þ 1)nc þ n equations. For the simultaneous solution strategy, the nonlinear algebraic equation solver subroutine NEQNF in IMSL (Fortran Math Library) is used to obtain the mole fractions of the gas at the inlet of the permeate side. Having obtained the mole fractions of the gas at the permeate side inlet, we then add 2n differential equations (Eqs. (1) and (2)) and solve the system of differential and algebraic equations using the DASSL software. 2.2. Model for the counter-current conﬁguration We consider the counter-current conﬁguration of the membrane shown earlier in Fig. 1. The model equations for the cocurrent case hold with the exception of the following changes; Eq. (2) becomes:

dGi ¼ Ni dA

Gi ðAT Þ ¼ 0

i ¼ 1; 2; n

(12)

For the counter-current case, the values of yi at the exit of the retentate side (inlet of permeate side) are unknown. These should be assumed by guessing the values of Fi(AT). Again for the solution strategy, the nonlinear algebraic equations solver NEQNF from IMSL is used to obtain the gas mole fractions on the permeate side inlet. After obtaining the gas mole fractions on the permeate side inlet, we subsequently add 2n differential equations (Eqs. (1) and (2)) and solve the system of differential and algebraic equations via the DASSL software, starting from the permeate inlet side (A ¼ AT); using the values of the assumed Fi(AT). At the exit of the retentate side (A ¼ 0), a total of (n) equations must be satisﬁed;

Fi ðcomputedÞ ¼ Fi ð0ÞðgivenÞ

(13)

These n equations in n unknowns Fi(AT) are iterated on in an external loop using NEQNF until convergence is reached. 3. Results and discussion 3.1. Validation study The model is ﬁrst solved and validated using the data pertinent to the separation of hydrogen from hydrocarbons, as reported in the experimental work of Rao and Sircar (Rao and Sircar, 1996). The nanomembrane has a thickness of 2.5 mm, a pore diameter of 5 A, a porosity of 0.36, and a tortuosity of 2. The values of Knudsen diffusivity, binary gas diffusivities, and viscosities are hence calculated (Poling et al., 2001). In the paper of Rao and Sircar, the membrane performance was evaluated in terms of hydrogen recovery, concentrations of gases in the permeate side as well as hydrocarbon rejections. The feed gas ﬂow rate was maintained constant at 0.067 gmol/s and it consisted (in mol %) of 40% H2, 20% CH4, 20% C2H6, 10% C3H8, and 10% C4H10. The temperature was kept constant at 263 K while the feed pressure was varied for a countercurrent conﬁguration model. Table 2 lists the model predictions together with the experimental results for the case of a sweep gas pressure of 1.07 atm and a hydrogen sweep gas consisting of 10% of the feed ﬂow rate. Four values of permeate pressure (PH) were investigated as: 5.11, 4.39, 3.38 and 1.35 atm. It can be seen from the table that, the model predictions follow the expected trend for the effect of increasing feed pressure (PH). The hydrogen recovery in the retentate stream decreases as PH increases, while the hydrogen composition increases. It is also noticed that the relative error between the predictions of the

1281

developed model and the experimental results is reasonable. The relative error reaches the value of around 16% for the prediction of hydrogen recovery for PH ¼ 5.11 atm, but the error is smaller (below 8%) for lower feed pressure. In a similar way, the relative error is below 7% for the predictions of hydrogen and methane compositions. As for the butane and propane, the relative error is larger. This can be attributed to the small values of their compositions. 3.2. Results for the nitrogenenatural gas separation The validated model is then used for the investigation of membrane performance for the nitrogen separation from natural gas. The nominal feed composition consists of 100 mol/hr of a mixture of nitrogen and natural gas with the following composition: 12.9% N2, 67.8% CH4, 30% C2H6, 10% C3H8, and 2% n-C4H10. The temperature is assumed to be constant at 54 C. In the ﬁrst set of investigation, the ﬂow conﬁguration is assumed to be co-current. Table 3 summarizes the composition of the gases at the exit of the membrane. As can be seen, the nitrogen recovery increases with permeate pressure. Nitrogen recovery is interpreted as the nitrogen fraction in the retentate stream. Starting from a value of 29.6% at a permeate pressure of 1 bar, the nitrogen recovery increases to 52.9% for a permeate pressure of 4 bar. The methane loss also increases from 21.5% to around 47.6%. The methane loss is deﬁned as the fraction of methane in the retentate stream. Table 3 also demonstrates that the permeate stream is rich in methane, where the mole fraction reaches 77%, while the nitrogen mole fraction constitutes about 13% of the stream. Moreover, the composition of the retentate displays a rich stream in methane, where its composition increases with increasing permeate pressure. The nitrogen fraction in the retentate stream decreases, on the other hand, with the permeate pressure from 17.4% to 15.2%. The developed model also allows a sensitivity analysis for the performance of the membrane. Fig. 2a depicts the variations of methane loss with the relative area for feed pressure of 10 bar and for different permeate pressure values 1, 2 and 4 bars. The relative area is deﬁned by s ¼ AQFLm PH , where Qm is the permeability of the base component (nitrogen). Given an assumed total area of the membrane of 20 m2, the maximum value of the relative area is 0.0235. It can be seen from the ﬁgure that, as expected, the methane loss decreases with the relative area of the membrane. Typical values of methane loss range from 0.1 to 0.8 for relative areas in the range of 0.01e0.02. In addition, the ﬁgure shows that for a desired methane loss, an increase in the permeate pressure would require a larger relative area of the membrane. As an example, for a desired methane loss of 60%, an increase in pressure from 1 bar to 4 bar would increase the relative area from 0.012 to 0.021. Nevertheless, Fig. 2b presents the effect of permeate pressure on the nitrogen recovery and its purity. As can be noted, for a required nitrogen recovery, an increase in the permeate pressure decreases the nitrogen purity accordingly. For example, at a gas pressure of 1 bar, a recovery of 60% is associated with a nitrogen purity of 0.17%, while at larger feed pressure of 4 bar, the purity decreases to 0.14%. The effect of permeate pressure on the decrease in nitrogen purity is clearer for smaller values of nitrogen recovery. For the same co-current conﬁguration, Fig. 3a demonstrates the effect of increasing the feed pressure on the performance of the nanomembrane. In this context, the permeate pressure is maintained at 1 bar. It is obvious that for the same area, an increase in the feed pressure entails a subsequent decrease in the methane loss. By way of illustration, for a relative area of 0.015, an increase in the feed pressure from 10 to 25 bar would decrease the methane loss from

1282

A.A. Al-Rabiah et al. / Journal of Natural Gas Science and Engineering 26 (2015) 1278e1284

Table 2 Comparison between experimental data and model predictions for the effect of feed gas pressure (sweep pressure maintained at 1.07 atm and ratio of hydrogen sweep to feed ﬂow rate is 0.1). Feed gas pressure (atm)

Results

H2 recovery (%)

H2 mol (%)

CH4 mol (%)

C2H6 mol (%)

C3H8 mol (%)

5.11 4.39 3.38 1.35 5.11 4.39 3.38 1.35 5.11 4.39 3.38 1.35

Experimental

62.5 78.5 80.1 98.4 72.80 78.6 86.5 99.7 16.5 0.1 8.0 1.3

57.0 52.1 49.5 42.6 53.4 52.0 49.4 43.7 6.3 0.2 0.2 2.6

26.3 25.3 23.2 21.1 26.3 25.3 23.7 20.1 0.0 0.0 2.2 4.7

14.5 17.7 19.5 19.5 16.8 17.8 18.6 18.9 15.9 0.6 4.6 3.1

2.4 0.0 4.5 0.4 6.5 1.3 8.7 8.0 3.3 0.08 4.5 0.43 6.1 2.2 8.8 8.5 37.5 e 0.0 7.5 6.2 69.2 1.1 6.3 Some values of relative errors are large due to small compositions

Model results

Relative error (%)

Observations

C4H10 mol (%)

Table 3 Effect of permeate pressure on the nanomembrane performance (Conditions of Fig. 2 at the relative area of 0.0239). Feed pressure

Permeate pressure

PH (bar)

PL (bar)

10 10 10

1 2 4

N2 recovery (%)

29.57 37.55 52.92

Methane loss (%)

21.46 30.02 47.57

Composition in permeate (%)

Composition in retentate (%)

N2

CH4

C2H6

C3H8

C4H10

N2

CH4

C2H6

C3H8

C4H10

13.12 13.08 13.13

76.90 77.00 76.85

5.62 5.60 5.63

2.21 2.19 2.22

2.15 2.13 2.17

17.38 16.38 15.19

66.24 68.79 71.75

7.79 7.27 6.66

3.97 3.55 3.06

4.62 4.02 3.34

(a)

(a)

0.8 Methane Loss

Methane Loss

0.8

0.6

0.4

0.2

4 bar 2 bar 1 bar

0.01

0.02 Relative Area

0.6

0.4 10 bar 15 bar

0.2

25 bar

0.01

0.03

0.02 Relative Area

(b)

(b)

0.8

Nitrogen Recovery

Nitrogen Recovery

0.8

0.6

0.4

0.2 0.14

0.03

4 bar 2 bar 1 bar

0.16 0.18 Nitrogen Purity

0.6

0.4 10 bar

0.2

0.2

Fig. 2. Effect of permeate pressure on the nanomembrane performance. Co-current conﬁguration. Porosity is 0.36. Feed pressure is 10 bar. Nitrogen in the feed is 14.14%.

0.14

15 bar 25 bar

0.16 0.18 Nitrogen Purity

0.2

Fig. 3. Effect of feed pressure on the nanomembrane performance. Co-current conﬁguration. Porosity is 0.36. Permeate pressure is 1 bar. Nitrogen in the feed is 14.14%.

A.A. Al-Rabiah et al. / Journal of Natural Gas Science and Engineering 26 (2015) 1278e1284

1283

(a)

0.8 Methane Loss

Methane Loss

0.8

0.6

0.4

0.36 0.036 0.0036 SD

0.2

0.6

0.4

0.2

cocurrent counter current

0.01

0.001 0.01 0.1 1 10 100 1000 Relative Area

0.02 Relative Area

0.03

(b)

0.6 to 0.55. In spite of that, Fig. 3b illustrates that for desired nitrogen purity, the increase in the feed pressure increases the nitrogen recovery. Hence, for nitrogen purity of 0.14, an increase in feed pressure values from 10, 15e25 bar increases the nitrogen recovery from 0.6 to 0.61 to 0.63. The pressure increase from 15 to 25 bar is noticed to be insigniﬁcant. The effect of porosity on the membrane performance is introduced as in Fig. 4. Smaller values of porosity would make the model approach the asymptotic simple solution-diffusion case. It can be realized from Fig. 4 that, the porosity has a substantial effect on the performance of the membrane. To give an instance, for a desired nitrogen recovery of 80%, a decrease in the porosity from 0.36 to 0.036 increases the required relative area from 0.001 to 0.1. The asymptotic case is the solution-diffusion (SD) model where the required area would be 500% more. Additionally, the effect of ﬂow conﬁguration on the membrane performance is examined. Table 4 displays the performance of the membrane for co and counter-current ﬂow conﬁgurations. The feed pressure is adjusted at 10 bar, while the permeate feed pressure is 2 bar. It appears that the counter-current ﬂow yields a larger nitrogen recovery and a slightly larger methane loss. As for the permeate stream, the methane mole fraction is larger for co-current ﬂow (77% compared to 75.62%). The nitrogen composition is, on the contrary, larger for the counter-current ﬂow. The composition of the rest of hydrocarbons is recognized to be larger in the counter-current case. As for the composition of the retentate stream, the table shows opposite trends to the permeate stream. The methane composition is larger in counter-current, while the opposite is for nitrogen composition. Contradictorily, the rest of hydrocarbons compositions are larger for co-current ﬂow. Another aspect of the effect of ﬂow conﬁguration is illustrated in Fig. 5(aeb). The feed pressure is maintained at 10 bar and the permeate pressure at 2 bar. It is found that for the same relative area, the counter-current

Nitrogen Recovery

Fig. 4. Effect of porosity on the nanomembrane performance. Co-current conﬁguration. Feed pressure is 10 bar. Permeate pressure is 2 bar. Nitrogen in the feed is 14.14%.

0.8

0.6 co current counter current

0.4

0.2 0.14

0.16 0.18 Nitrogen Purity

0.2

Fig. 5. Effect of ﬂow conﬁguration on the nanomembrane performance. Porosity is 0.36. Feed pressure is 10 bar. Permeate pressure is 2 bar. Nitrogen in the feed is 14.14%.

conﬁguration yields relatively smaller methane loss (see Fig. 5a). For a relative area of 0.01, the methane loss is 70% with countercurrent, compared to 69% for co-current conﬁguration. Nonetheless, the effect of ﬂow conﬁguration is evidently clearer in Fig. 5b. It can be perceived that, for a desired nitrogen purity, the countercurrent ﬂow yields larger nitrogen recovery. In the manner that, for a nitrogen purity of 0.15, the counter-current ﬂow conﬁguration would yield a nitrogen recovery of 80% compared to only 79% for co-current ﬂow. The effect of the ﬂow conﬁguration is more accentuated when smaller nitrogen purity (i.e. high nitrogen recovery) is sought. 4. Conclusions This paper has developed a ﬁrst principle model for the separation of gases in carbon nanomembranes. The model is based on the classical dusty gas model coupled with a simple surface diffusion model. In the ﬁrst stage, the developed model was validated against the experimental work in the literature for the separation of hydrogen from hydrocarbons. The model was later used for a

Table 4 Effect of ﬂow conﬁguration pressure on the nanomembrane performance (Conditions of Fig. 5 at the relative area of 0.0239). Flow conﬁguration

Co-current Counter-current

N2 recovery (%)

37.55 85.36

Methane loss (%)

30.02 30.76

Composition in permeate (%)

Composition in retentate (%)

N2

CH4

C2H6

C3H8

C4H10

N2

CH4

C2H6

C3H8

C4H10

13.08 13.69

77.00 75.62

5.60 5.90

2.19 2.22

2.13 2.40

16.38 14.58

68.79 73.34

7.27 6.35

3.55 2.78

4.02 2.94

1284

A.A. Al-Rabiah et al. / Journal of Natural Gas Science and Engineering 26 (2015) 1278e1284

theoretical investigation of the nanomembrane performance for the nitrogen separation from natural gas. The study examined the performance of the membrane for nominal industrial values of feed conditions. The model also enabled performing useful parametric study of the effect of various operating parameters on the membrane performance, including the effect of feed pressure, permeate pressure as well as ﬂow conﬁguration. The model developed in this study is general and can also be applied to different kinds of nanoporous membrane ﬂow patterns. Acknowledgments The authors gratefully acknowledge ﬁnancial support from King Abdullah Institute for Nanotechnology at King Saud University, Riyadh. References Ahmad, F., Keong, L.K., Mun, S.S., Raﬁq, S., Khan, A.U., Lee, M., 2015. Hollow ﬁber membrane model for gas separation: process simulation, experimental validation and module characteristics study. J. Ind. Eng. Chem. 21, 1246e1257. http://dx.doi.org/10.1016/j.jiec.2014.05.041. €o € k, M., Jakobsson, K., Lardelli, M., Snowden, S., So € derbergh, B., 2010. Aleklett, K., Ho The peak of the oil age e analyzing the world oil production reference scenario in world energy outlook 2008. Energy Policy 38, 1398e1414. http://dx.doi.org/ 10.1016/j.enpol.2009.11.021. Baker, R.W., 2002. Future directions of membrane gas separation technology. Ind. Eng. Chem. Res. 41, 1393e1411. http://dx.doi.org/10.1021/ie0108088. Baker, R.W., Lokhandwala, K.A., Wijmans, J.G., Costa, A.R. Da, 2003. Nitrogen removal from natural gas using two types of membranes. U.S. Patent 6,630,011. Bara, J.E., Gabriel, C.J., Carlisle, T.K., Camper, D.E., Finotello, A., Gin, D.L., Noble, R.D., 2009. Gas separations in ﬂuoroalkyl-functionalized room-temperature ionic liquids using supported liquid membranes. Chem. Eng. J. 147, 43e50. http:// dx.doi.org/10.1016/j.cej.2008.11.021. Bowen, W.R., Welfoot, J.S., 2002. Modelling the performance of membrane nanoﬁltration-critical assessment and model development. Chem. Eng. Sci. 57, 1121e1137. http://dx.doi.org/10.1016/S0009-2509(01)00413-4. Cai, J.J., Hawboldt, K., Abdi, M.A., 2012. Contaminant removal from natural gas using dual hollow ﬁber membrane contactors. J. Memb. Sci. 397e398, 9e16. http:// dx.doi.org/10.1016/j.memsci.2011.12.017. Dionysiou, D.D., 2004. Environmental applications and implications of nanotechnology and nanomaterials. J. Environ. Eng. 130, 723e724. http://dx.doi.org/ 10.1061/(ASCE)0733-9372(2004)130:7(723). Fuertes, A.B., 2000. Adsorption-selective carbon membrane for gas separation. J. Memb. Sci. 177, 9e16. http://dx.doi.org/10.1016/S0376-7388(00)00458-0. Habib, K., Habib, A., 2004. General model of hydrogen transport through nanoporous membranes. Compos. Part B Eng 35, 191e195. http://dx.doi.org/10.1016/ j.compositesb.2003.08.007. Koresh, J.E., Sofer, A., 1983. Molecular sieve carbon permselective membrane. Part I. Presentation of a new device for gas mixture separation. Sep. Sci. Technol. 18, 723e734. http://dx.doi.org/10.1080/01496398308068576. Lokhandwala, K.A., Pinnau, I., He, Z., Amo, K.D., DaCosta, A.R., Wijmans, J.G., Baker, R.W., 2010. Membrane separation of nitrogen from natural gas: a case study from membrane synthesis to commercial deployment. J. Memb. Sci. 346, 270e279. http://dx.doi.org/10.1016/j.memsci.2009.09.046. Mulder, M., 1996. Basic Principles of Membrane Technology. Springer Science & Business Media. Poling, B.E., Prausnitz, J.M., O’connell, J.P., 2001. The Properties of Gases and Liquids, ﬁfth. ed. McGraw-Hill, New York. Rao, M.B., Sircar, S., 1993a. Nanoporous carbon membrane for gas separation. Gas. Sep. Purif. 7, 279e284. http://dx.doi.org/10.1016/0950-4214(93)80030-Z. Rao, M.B., Sircar, S., 1993b. Nanoporous carbon membranes for separation of gas mixtures by selective surface ﬂow. J. Memb. Sci. 85, 253e264. http://dx.doi.org/ 10.1016/0376-7388(93)85279-6. Rao, M.B., Sircar, S., 1996. Performance and pore characterization of nanoporous carbon membranes for gas separation. J. Memb. Sci. 110, 109e118. http:// dx.doi.org/10.1016/0376-7388(95)00241-3. Rezakazemi, M., Niazi, Z., Mirfendereski, M., Shirazian, S., Mohammadi, T., Pak, A., 2011. CFD simulation of natural gas sweetening in a gas-liquid hollow-ﬁber membrane contactor. Chem. Eng. J. 168, 1217e1226. http://dx.doi.org/10.1016/ j.cej.2011.02.019. Rufford, T.E., Smart, S., Watson, G.C.Y., Graham, B.F., Boxall, J., Diniz da Costa, J.C., May, E.F., 2012. The removal of CO2 and N2 from natural gas: a review of conventional and emerging process technologies. J. Pet. Sci. Eng. 94e95, 123e154. http://dx.doi.org/10.1016/j.petrol.2012.06.016. Saidi, M., Heidarinejad, S., Rahimpour, H.R., Talaghat, M.R., Rahimpour, M.R., 2014.

Mathematical modeling of carbon dioxide removal using amine-promoted hot potassium carbonate in a hollow ﬁber membrane contactor. J. Nat. Gas. Sci. Eng 18, 274e285. http://dx.doi.org/10.1016/j.jngse.2014.03.001. Scholes, C.A., Stevens, G.W., Kentish, S.E., 2012. Membrane gas separation applications in natural gas processing. Fuel 96, 15e28. http://dx.doi.org/10.1016/ j.fuel.2011.12.074. Seo, Y.G., Kum, G.H., Seaton, N.A., 2002. Monte Carlo simulation of transport diffusion in nanoporous carbon membranes. J. Memb. Sci. 195, 65e73. http:// dx.doi.org/10.1016/S0376-7388(01)00549-X. Shindo, Y., Hakuta, T., Yoshitome, H., Inoue, H., 1985. Calculation methods for multicomponent gas separation by permeation. Sep. Sci. Technol. 20, 445e459. http://dx.doi.org/10.1080/01496398508060692. Soliman, M.A., 1992. A spline collocation method for the solution of diffusionconvection problems with chemical reactions. Chem. Eng. Sci. 47, 4209e4213. Tagliabue, M., Farrusseng, D., Valencia, S., Aguado, S., Ravon, U., Rizzo, C., Corma, A., Mirodatos, C., 2009. Natural gas treating by selective adsorption: material science and chemical engineering interplay. Chem. Eng. J. 155, 553e566. http:// dx.doi.org/10.1016/j.cej.2009.09.010. Vieira-Linhares, A.M., Seaton, N.A., 2003. Non-equilibrium molecular dynamics simulation of gas separation in a microporous carbon membrane. Chem. Eng. Sci. 58, 4129e4136. http://dx.doi.org/10.1016/S0009-2509(03)00304-X. Wijmans, J.G., Baker, R.W., 1995. The solution-diffusion model: a review. J. Memb. Sci. 107, 1e21. http://dx.doi.org/10.1016/0376-7388(95)00102-I. Wu, T., Diaz, M.C., Zheng, Y., Zhou, R., Funke, H.H., Falconer, J.L., Noble, R.D., 2015. Inﬂuence of propane on CO2/CH4 and N2/CH4 separations in CHA zeolite membranes. J. Memb. Sci. 473, 201e209. http://dx.doi.org/10.1016/ j.memsci.2014.09.021. Xu, L., Sedigh, M.G., Tsotsis, T.T., Sahimi, M., 2000. Nonequilibrium molecular dynamics simulation of transport and separation of gases in carbon nanopores. II. Binary and ternary mixtures and comparison with the experimental data. J. Chem. Phys. 112, 910e922. http://dx.doi.org/10.1063/1.480618. € Kiss, A.A., Hüser, N., Leßmann, K., Kenig, E.Y., 2012. Reactive absorption Yildirim, O., in chemical process industry: a review on current activities. Chem. Eng. J. 213, 371e391. http://dx.doi.org/10.1016/j.cej.2012.09.121.

Nomenclature A: membrane area (m2) AT: total membrane area (m2) Aj,k: elements of the matrix of the weights of ﬁrst derivative DK: Knudsen diffusivity (m2/s) Dij: binary gas diffusivity (m2/s) F: inlet feed ﬂowrate (mol/s) G: ﬂowrate in permeate (mol/s) L: membrane thickness (m) M: mole fractions at the permeate side N: number of components nc: number of collocation points N: dusty ﬂux (mol/m2s) NSD: surface diffusion ﬂux (mol/m2s) NT: total ﬂux through the membrane (mol/m2s) P: total pressure inside the membrane (Pa) PF: feed pressure (Pa) PH: pressure on feed side (Pa) PP: pressure on permeate side (Pa) Q: permeability (mol/s.m.Pa) r: pore radius (m) R: universal gas constant (J/mol K) s: dimensionless relative area T: temperature (K) x: mole fraction inside the membrane Xinterp: vector of weights of the Lagrange interpolation y: gas mole fraction at the permeate side z: dimensionless distance through the membrane Greek ε: porosity m: gas viscosity (kg/m.s) t: turtosity Subscripts i,j,k: component index M: base component F: feed H: feed side P: permeate side

Copyright © 2020 COEK.INFO. All rights reserved.